Abstract
Tetragonal ferroelectric/ferroelectricsuperlattice under uniaxial tensile stress along the c axis is investigated from first principles. We show that the calculated ideal tensile strength is 6.85 GPa and that the superlattice under the loading of uniaxial tensile stress becomes soft along the nonpolar axes. We also find that the appropriately applied uniaxial tensile stress can significantly enhance the piezoelectricity for the superlattice, with piezoelectric coefficient d_{33} increasing from the ground state value by a factor of about 8, reaching 678.42 pC/N. The underlying mechanism for the enhancement of piezoelectricity is discussed.
Keywords:
Mechanical property; Piezoelectricity; Ferroelectric superlatticeIntroduction
Ferroelectrics, which can convert mechanical to electrical energy (and vice versa) have wide applications in medical imaging, telecommunication and ultrasonic devices, the physical properties of which are sensitive to external conditions, such as strain, film thickness, temperature, electric and magnetic fields [13]. BaTiO_{3} (BTO) and PbTiO_{3} (PTO), as prototype ferroelectric materials and simple systems, have been intensively studied [4,5]. It is known that the ferroelectricity arises from the competition of shortrange repulsions which favor the paraelectric cubic phase and Coulomb forces, which favor the ferroelectric phase [6,7]. As the pressure increases, the shortrange repulsions increase faster than the Coulomb forces, leading to the reduced ferroelectricity. Accompanied with the suppression of ferroelectricity, the piezoelectricity decreases and even disappears. However, recent studies have shown that the noncollinear polarization rotation, occurring at phase transition pressure, can result in the giant piezoelectric response [8,9]. In contrast to previous theoretical studies of the effects of epitaxial strain on the spontaneous polarization of ferroelectric thin films, we have systematically studied the influence of uniaxial and inplane epitaxial strains on the mechanical and piezoelectric properties of perovskite ferroelectrics [1015]. So far, there has been no previous work on the effect of uniaxial tensile strains on the mechanical and piezoelectric properties of shortperiod BTO/PTO superlattices.
Ferroelectric superlattices composed of alternating epitaxial oxides ultrathin layers are currently under intensive study due to their excellent ferroelectric and piezoelectric properties [16]. Ferroelectricity can be induced in superlattice in spite of the paraelectric nature of and . This is because the coincidence of the positive and negative charge centers is destroyed in the superlattice and electric dipoles are induced. Moreover, ferroelectricity can be enhanced in ferroelectric superlattices in certain stacking sequences [17]. The overall polarization of threecomponent SrTiO_{3}(STO)/BTO/PTO ferroelectric superlattices can also be improved by increasing the number of BTO and PTO layers [18]. Thanks to the periodic nature, it is possible to study the effect of uniaxial or biaxial strains on the properties of ferroelectric superlattices from first principles.
In this work, we perform total energy as well as linear response calculations to study the effect of uniaxial tensile stress along the c axis on the mechanical and piezoelectric properties of shortperiod BTO/PTO superlattice. We show the mechanical properties by calculating the ideal tensile strength, elastic constants and valence charge density at different strains. We also show the influence of uniaxial stress on the piezoelectricity. To reveal the underlying mechanisms, we study the effects of uniaxial tensile stress on the atomic displacements and Born effective charges, respectively.
Computational Methods
Our calculations are performed within the local density approximation (LDA) to the density functional theory (DFT) as implemented in the planewave pseudopotential ABINIT package [19]. To ensure good numerical convergence, the planewave energy cutoff is set to be 80 Ry, and the Brillouin zone integration is performed with 6 × 6 × 6 kmeshpoints. The normconserving pseudopotentials generated by the OPIUM program are tested against the allelectron fullpotential linearized augmented planewave method [20,21]. The orbitals of Ba 5s^{2}5p^{6}6s^{2}, Pb 5d^{10}6s^{2}6p^{2}, Ti 3s^{2}3p^{6}3d^{2}4s^{2} and O 2s^{2}2p^{4} are explicitly included as valence electrons. The dynamical matrices and Born effective charges are computed by the linear response theory of strain type perturbations, which has been proved to be highly reliable for ground state properties [2224]. The polarization is calculated by the Berryphase approach [25]. The LDA is used instead of the generalized gradient approximation (GGA) because the GGA is found to overestimate both the equilibrium volume and strain for the perovskite structures [26]. The piezoelectric strain coefficients , where e is the piezoelectric stress tensor and the elastic compliance tensor s is the reciprocal of the elastic stiffness tensor c (Roman indexes from 1 to 3, and Greek ones from 1 to 6).
In the calculations, a doubleperovskite tenatom supercell along the c axis is used for the tetragonal shortperiod BTO/PTO superlattice. The primitive periodicity of tetragonal structure with the space group P4mm is retained, which is more stable in energy than the rhombohedral structure. For the tetragonal perovskite structure compounds BTO and PTO, the equilibrium lattice parameters are a(BTO)=3.915and, which are slightly less than the experimental values of 3.994, 4.034, 3.904 and, respectively [13,14]. A sketch of ground state shortperiod BTO/PTO superlattice with its atomic positions is shown in Fig. 1.
Figure 1. The sketch of shortperiod ferroelectric superlattice with its atomic positions
To calculate the uniaxial tensile stress σ_{33}, we apply a small strain increment η_{3} along the c axis and then conduct structural optimization for the lattice vectors perpendicular to the c axis, and all the internal atomic positions until the two components of stress tensor (i.e., σ_{11} and σ_{22}) are smaller than 0.05 GPa. The strain is then increased step by step. Since, the elastic constants satisfy η_{3}/η_{1}≈ − (c_{11} + c_{12})/c_{13} under the loading of uniaxial tensile strain applied along the c axis, where the strains η_{i} are calculated by η_{1} = η_{2} = (a − a_{0})/a_{0} and η_{3} = (c − c_{0})/c_{0}, withandbeing the lattice constants of the unstrained superlattice structure. We have examined the accuracy of our calculations by studying the influence of different strains on the properties of BTO and PTO, respectively [1215].
Results and Discussion
Figure 2a shows the uniaxial tensile stress σ_{33} as a function of strain η_{3}. The relation between strains η_{1} and η_{3} is shown in the inset, which satisfy η_{3} > −2η_{1}. The stress σ_{33} increases until reaching its maximum value of 6.85 GPa with increasing strain, indicating that the calculated ideal tensile strength is 6.85 GPa for the superlattice, which is the maximum stress required to break the superlattice. Figure 2b shows the elastic constants as a function of stress σ_{33}, which reflect the relation between stress and strain. What is the most unexpected is that the constant c_{33} first decreases until reaching its minimum value at σ_{c} = 3.26 GPa and then gradually increases, promising a large electromechanical response at σ_{c}[27]. The minimum c_{33} corresponds to the minimum slope of the curve of Fig. 2a at σ_{c}. Other elastic constants, especially c_{11}, always decrease with increasing σ_{33}, indicating that the superlattice under the loading of uniaxial tensile stress along the c axis becomes soft along the nonpolar axes.
Figure 2. a Uniaxial tensile stress as a function of tensile strain η_{3}, and the inset reflects the relation between strains η_{3} and η_{1}. b Elastic constants as a function of stress σ_{33}
To illustrate the change of chemical bonds with uniaxial tensile stress, Fig. 3a and 3b are plotted to show the valence charge density along the c axis in the (100) and (200) planes of the superlattice at equilibrium, maximum piezoelectric coefficient and ideal tensile strength, respectively. The Pb − O_{4}, Ba − O_{1}, Ti_{1}O_{1} and Ti_{2}O_{4} bond lengths are not sensitive to the uniaxial tensile stress along the c axis, suggesting that the orbital hybridizations between these atoms are not sensitive to the uniaxial strain, whereas the Ti_{1}O_{3} and Ti_{2}O_{6} bonds elongate remarkably with increasing stress. Following the evolution of the charge density, we find that the weak Ti_{1}O_{3} bond starts to break first, followed by the Ti_{2}O_{6} bond. After the bond breaks, the system converts into a planar structure with alternating layers. On the other hand, Fig. 3a and 3b show that the valence charge density becomes more and more unsymmetrical with the uniaxial tensile stress increasing, indicating the increase in polarization. To confirm this, we have directly calculated the relations between the polarization and the uniaxial tensile stress with the Berryphase approach.
Figure 3. Calculated valence charge density along the c axis in the (100) (a) and (200) (b) planes of superlattice at equilibrium (1), maximum piezoelectric coefficient (2) and ideal tensile strength (3)
Figure 4a shows the polarization as a function of uniaxial tensile stress. For the ground state superlattice, the calculated spontaneous polarization of 0.29 C/m^{2} is less than the theoretical value of 0.81 C/m^{2} of ground state PTO, but slightly larger than the value of 0.28 C/m^{2} of tetragonal BTO (the other theoretical value is 0.26 C/m^{2}[28]), which supports the conclusion that the sharp interfaces suppress the polarization in shortperiod BTO/PTO superlattices [28]. As the stress σ_{33} increases, the polarization dramatically increases with the maximum slope appearing at σ_{c}, indicating that the ferroelectric phase becomes more and more stable with respect to the paraelectric phase. Figure 4b shows the variation of piezoelectric coefficients with stress σ_{33}, which are calculated by the linear response theory. The piezoelectric coefficients all increase with increasing σ_{33} and reach their maximum values at σ_{c}, indicating that the appropriately applied uniaxial tensile stress can enhance the piezoelectricity for the superlattice. The piezoelectric coefficient d_{33} of ground state superlattice is 86.36 pC/N, which is slightly less than the value of 103.18 pC/N of PTO, but much larger than the value of 36.43 pC/N of BTO. Under the loading of uniaxial tensile stress applied along the c axis, d_{33} is increased from its ground state value by a factor of about 8, reaching 678.42 pC/N for the superlattice. From previous calculations [14], we know that the uniaxial tensile stress can only enhance d_{33} of PTO to the maximum value of 380.50 pC/N. The enhancement of piezoelectricity is supported by the conclusion of uniaxial tensile stress dependency of elastic constant c_{33} (see Fig. 2b). Note that the polarization under uniaxial stress remains along the <001> direction and that the piezoelectric coefficients reflect the slope of polarization versus stress curves. The enhancement of piezoelectricity corresponds to the maximum slope of the curve of Fig. 4a at σ_{c}, it is the change of magnitude of polarization that leads to the enhancement of piezoelectricity.
Figure 4. Uniaxial tensile stress dependence of a polarization and b piezoelectric coefficients (i.e.,d_{31} and d_{33})
To reveal the underlying mechanisms for the abnormal piezoelectricity, we study the effects of uniaxial tensile stress on the Born effective charges and atomic displacements, respectively (see Fig. 5a, 5b). Since the atomic displacements and polarization are all along the c axis, only charges Z_{zz}^{*} contribute to the polarization. The uniaxial tensile stress reduces the effective charges, which remain almost constant when σ_{33} > σ_{c}. The charges Z_{zz}^{*} of O_{1} and O_{4} atoms are much close to their normal charges, so does the case of Ti atoms when σ_{33} > σ_{c}, whereas Z_{zz}^{*} of O_{3} and O_{6} atoms are anomalously large compared with their normal charges, suggesting the strong orbital hybridization between Ti_{1}(and Ti_{2}) 3d and O_{6}(and O_{3}) 2p states (see Fig. 3b). Note that the Ba atom is fixed at (0, 0, 0) during the firstprinciples simulations. The displacements of O atoms, which are much larger than those of Pb and Ti atoms for a broad range of stress, are greatly enhanced as the stress σ_{33} increases, especially near σ_{c}, leading to the drastic increase in polarization. It is concluded that as the stress σ_{33} increases, the atomic displacements are so greatly enhanced that the overall effect is the increase in polarization, even though the magnitudes of Z_{zz}^{*} decrease with the stress increasing.
Figure 5. a Born effective charges Z_{zz}^{*} and b atomic displacements along the c axis (in c units), relative to the centrosymmetric reference structure, as a function of uniaxial tensile stress
Summary
In summary, we have studied the influence of uniaxial tensile stress applied along the c axis on the mechanical and piezoelectric properties of shortperiod BTO/PTO superlattice using firstprinciples methods. We show that the calculated ideal tensile strength is 6.850 GPa and that the superlattice under the loading of uniaxial tensile stress becomes soft along the nonpolar axes. We also find that the appropriately applied uniaxial tensile stress can significantly enhance the piezoelectricity for the superlattice. Our calculated results reveal that it is the drastic increase in atomic displacements along the c axis that leads to the increase in polarization and that the enhancement of piezoelectricity is attributed to the change in the magnitude of polarization with the stress. Our work suggests a way of enhancing the piezoelectric properties of the superlattices, which would be helpful to enhance the performance of the piezoelectric devices.
Acknowledgments
The work is supported by the National Natural Science Foundation of China under Grant Nos. 10425210, 10832002 and 10674177, the National Basic Research Program of China (Grant No. 2006CB601202), and the Foundation of China University of Mining and Technology.
Open Access
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.
References

Lines ME, Glass AM: Principles and Applications of Ferroelectrics and Telated Materials. Clarendon, Oxford; 1979.

Uchino K: Piezoelectric Actuators and Ultrasonic Motors. Kluwer, Boston; 1996.

Zhu Z, Zhang H, Tan M, Zhang X, Han J:
J. Phys. D: Appl. Phys.. 2009, 41:215408.
Bibcode number [2008JPhD...41u5408Z]
Publisher Full Text 
Zhong W, Vanderbilt D, Rabe KM:
Phys. Rev. B. 1995, 52:6301.
COI number [1:CAS:528:DyaK2MXotVSls7o%3D]; Bibcode number [1995PhRvB..52.6301Z]
Publisher Full Text 
Salehi H, Shahtahmasebi N, Hosseini SM:
Eur. Phys. J. B. 2003, 32:177.
COI number [1:CAS:528:DC%2BD3sXjs1ygtbY%3D]; Bibcode number [2003EPJB...32..177S]
Publisher Full Text 
Samara GA, Sakudo T, Yoshimitsu K:
Phys. Rev. Lett.. 1975, 35:1767.
COI number [1:CAS:528:DyaE28XmvVSkuw%3D%3D]; Bibcode number [1975PhRvL..35.1767S]
Publisher Full Text 
Nature. 1992, 358:136.
COI number [1:CAS:528:DyaK38Xlt1amtL4%3D]; Bibcode number [1992Natur.358..136C]
Publisher Full Text 
Nature. 2000, 403:281.
COI number [1:CAS:528:DC%2BD3cXns1CisA%3D%3D]; Bibcode number [2000Natur.403..281F]
PubMed Abstract  Publisher Full Text 
Phys. Rev. Lett.. 2005, 95:037601.
Bibcode number [2005PhRvL..95c7601W]
PubMed Abstract  Publisher Full Text 
Chin. Phys. Lett.. 2008, 25:1113.
COI number [1:CAS:528:DC%2BD1cXksFSgs7o%3D]; Bibcode number [2008ChPhL..25.1113S]
Publisher Full Text 
Phys. Rev. Lett.. 2005, 95:257601.
Bibcode number [2005PhRvL..95y7601E]
PubMed Abstract  Publisher Full Text 
Duan Y, Li J, Li SS, Xia JB, Chen C:
J. Appl. Phys.. 2008, 103:083713.
Bibcode number [2008JAP...103h3713D]
Publisher Full Text 
Chin. Phys. Lett.. 2009, 26:017203.
Bibcode number [2009ChPhL..26a7203W]
Publisher Full Text 
J. Phys.: Condens. Matter. 2008, 20:175210.
Bibcode number [2008JPCM...20q5210D]
Publisher Full Text 
Duan Y, Qin L, Tang G, Chen C:
J. Appl. Phys.. 2009, 105:033706.
Bibcode number [2009JAP...105c3706D]
Publisher Full Text 
J. Appl. Phys.. 2008, 104:126106.
Bibcode number [2008JAP...104l6106L]
Publisher Full Text 
Appl. Phys. Lett. 2003, 82:1586.
COI number [1:CAS:528:DC%2BD3sXhvV2ltrc%3D]; Bibcode number [2003ApPhL..82.1586N]
Publisher Full Text 
Shah SH, Bristowe PD, Kolpak AM, Rappe AM:
J. Mater. Sci.. 2008, 43:3750.
COI number [1:CAS:528:DC%2BD1cXlslajsLs%3D]; Bibcode number [2008JMatS..43.3750S]
Publisher Full Text 
Gonze X, Beuken JM, Caracas R, Detraux F, Fuchs M, Rignanese GM, Sindic L, Verstraete M, Zerah G, Jollet F, Torrent M, Roy A, Mikami M, Ghosez Ph, Raty JY, Allan DC:
Comput. Mater. Sci.. 2002, 25:478. Publisher Full Text

Rappe AM, Rabe KM, Kaxiras E, Joannopoulos JD:
Phys. Rev. B. 1990, 41:1227.
Bibcode number [1990PhRvB..41.1227R]
Publisher Full Text 
Singh DJ: Planewaves, Pseudopotential, and the LAPW Method. Kluwer, Boston, MA; 1994.

Phys. Rev. B. 1997, 55:10355.
COI number [1:CAS:528:DyaK2sXivFOlsbs%3D]; Bibcode number [1997PhRvB..5510355G]
Publisher Full Text 
Baroni S, de Gironcoli S, Dal Corso A, Giannozzi P:
Rev. Mod. Phys.. 2001, 73:515.
COI number [1:CAS:528:DC%2BD3MXlvFKrtLc%3D]; Bibcode number [2001RvMP...73..515B]
Publisher Full Text 
Hamann DR, Wu X, Rabe KM, Vanderbilt D:
Phys. Rev. B. 2005, 71:035117.
Bibcode number [2005PhRvB..71c5117H]
Publisher Full Text 
Phys. Rev. B. 1993, 47:1651.
COI number [1:CAS:528:DyaK3sXlvFeiu7o%3D]; Bibcode number [1993PhRvB..47.1651K]
Publisher Full Text 
Phys. Rev. B. 2004, 70:104112.
Bibcode number [2004PhRvB..70j4112W]
Publisher Full Text 
Phys. Rev. B. 2008, 77:045213.
Bibcode number [2008PhRvB..77d5213A]
Publisher Full Text 
Phys. Rev. B. 2009, 79:180101.
Bibcode number [2009PhRvB..79r0101C]
Publisher Full Text